Intermediate band electron wave function localization ... Intermediate band electron wave function...
Embed Size (px)
Transcript of Intermediate band electron wave function localization ... Intermediate band electron wave function...
Intermediate band electronwave function localization effect on the efficiency limits of InAs/GaAs quantum dot solar cell
Amir Mehdipour, Matsuto Ogawa, and Satofumi Souma
Department of Electrical and Electronic Engineering, Kobe University, 1-1 Rokkodai, Nada, Kobe 657-8501, Japan
Keywords: Intermediate Band Solar Cell, Quantum Dots, Tight-Binding Method
In the conventional detailed balance theory of quantum dot intermediate band solar cell (QD-IBSC), the electron wave function is assumed to be completely delocalized. Such wavefunctions are known to reduce thermal losses and enhance the photon-harvesting efficiency of an intermediate band. The aim of this study is to investigate the accuracy of the assumption of such “metallic-like IB” in determining the efficiency of IBSC in the presence of one or two IBs. According to our calculations for cubic model QD structures based on the finite element method, the electronic wave functions are strongly concentrated in the QD regions for the realistic QD spacing. The influence of such electron localization effects on the cell efficiency is then carefully examined by introducing the effective electron filling factor along with the detailed balance theory, with particular attention given to the roles played by the number of IBs and sunlight concentration. While the electron localization in IBs is detrimental for cell efficiency, the use of IBs is demonstrated to be still beneficial and improve the efficiency significantly under full sunlight concentration.
1. Introduction Luque and Marti showed that the introduction of an intermedi- ate band (IB) in the band gap of a regular semiconductor en- ables the absorption of two “below the gap photons” via the IB in a two-step process. In other words, electrons can be ex- cited from the valence band (VB) to the conduction band (CB) via the IBs in a multiple excitation process, as well as via the direct excitation path. For this mechanism, the detailed bal- ance theory predicts that the maximum efficiency of the solar cell (SC) can be up to 63.1% for an IBSC with a single IB. This compares favorably with the Shockley–Queisser (SQ) ef- ficiency limit of 40.7% under the maximum concentration of sunlight (46000 suns) for a single junction SC1, 2, 3). The IBSC can be achieved using materials that have intrinsic IBs between VB and CB4, 5) or by forming the IB by quantum-dot superlat- tices (QDSLs) inside conventional semiconductors. The latter scheme is called the quantum dot intermediate band solar cells (QD-IBSCs)6, 7, 8, 9, 10). Generally, a QD-IBSC structure is fabricated by sandwich- ing the QDSLs inside thep-n junction, as shown in Fig. 1. One-dimensionally ordered QDSLs with closely spaced QDs in thez direction is believed to allow QD electron wave func- tions to overlap and form the desired IB or IBs. There have been several experimental reports of vertical one-dimensional structures11, 12), as well as three-dimensional ones13, 14, 15), followed by the recent successful fabrication of a QD-IBSC module16, 17). Further progress in self-assembly growth is ex- pected to result in well-ordered QDSLs with closely spaced QDs to form better IBs. In this structure, inserting two layers
of conventional semiconductors between the stack of QD lay- ers and the electrodes is beneficial to sustain the flat-band po- tential in the QDSL region and maximize the effect of the QD layers (Fig. 1). Without the semiconductor layers, although the QDSL region is doped to make the IB half filled with electrons through modulation doping at the barrier region, IBs in some QD layers close to thep-type region become empty and to the n-type region become full. Thus, some QD layers do not con- tribute to the transitions through IBs without those additional layers8). The ideal IBSC with a single IB with completely delocalized electron wave function and infinitesimal bandwidth has been evaluated thus far by many researchers who suggest that a completely delocalized IB wave function is necessary to re- duce thermal losses and to enhance the photon-harvesting ef- ficiency of an intermediate band (IB)18, 6, 19, 20, 21). In reality, however, electron wave function is not completely delocalized but is rather localized inside QDs to some extent, with the ex- tent of such localization varying for the different IBs in the case of multiple IBs. Moreover, understanding the impact of the sunlight concentration on the efficiency limit of QD-IBSC is of interest when the electron wave-function localization ef- fect mentioned above is considered. Motivated by these considerations, we perform a numerical study of the influence of electron wave-function localization on the efficiency limit of QD-IBSC, with a special focus on the roles played by the number of IBs and the sunlight concentra- tion. While there have been several reports on ideal QD-IBSC with multiple IBs22, 23, 24), in this study, we focus on the influ- ence of non ideality in QD-IBSC caused by IB wave-function
(Received May 22, 2014; Accepted September 30, 2014; Online published November 21, 2014)
Memoirs of the Graduate Schools of Engineering and System Informatics Kobe University No. 6, pp. 18–24, 2014. doi:10.5047/gseku.e.2014.003
localization. We studythe dependence of the efficiency limits on the extent of the IB wave-functions for the case of concen- trated and unconcentrated sunlight illuminations. The paper is organized as follows. In the next section, we dis- cuss the QD-IBSC structure models and their electronic prop- erties. In Sec. III, we present the discussion of the detailed balance efficiency. In Sec. IV, we summarize our findings.
Figure 1: Simplified structure andband diagram of QD-IBSC with two field-damping layers.
2. Structure model and electronic properties 2.1. Structure models
In this study, we consider the QDSLs made of InAs QDs em- bedded in a GaAs barrier, which can be obtained experimen- tally by the self-assembly process. For the theoretical analy- sis of the efficiency in such InAs/GaAs based QD-IBSC, first, understanding the electronic energy eigenstates of electrons confined in such QDSLs by solving the three-dimensional effective-mass equations is necessary. Here, note that the actual self-assembled quantum dots are grown on the wetting layer (WL) that behaves like a quantum well with additional levels close to the CB minimum in the barrier material. As a consequence, the edge of the CB is lowered to the WL level25), leading to the reduction of the bandgap in the barrier material from the original 1.43 eV GaAs value to∼ 1.3 eV at room tem- perature, as reported in Ref.6). We use this reduced bandgap concept in our model to estimate the efficiency limit. Then, neglecting the strain and using the valence band offset of 0.17 eV 26) and the InAs band gap of 0.36 eV, the CB offset (i.e., the QD potential height in the CB) is estimated to be 0.77 eV. While strain has been suggested to cause the reduction of the CB offset27), in this study, we first neglect this effect because of our focus on qualitative understanding. We then comment on the effects of strain in our discussion of the numerical re- sults. Once the potential height is known, we can solve the CB effec- tive mass equation (Schrödinger equation) for understanding the energy eigenstates of the electrons confined in the QD,
HΨ(r) = EΨ(r), (1)
H = −∇ ℏ 2
2m∗(r) ∇+ V (r), (2)
where2πℏ is the Planck’sconstant, andm∗(r) andV (r) are the effective mass and the QDSL confinement potential, re- spectively, given bym∗ = 0.024m0 andV (r) = 0 inside the InAs QD, and bym∗ = 0.067m0 andV (r) = 0.77 eV outside the QD (i.e., in the GaAs region), withm0 being the free elec- tron mass. While the methodology presented below is valid, independent of the details of the geometrical structure of each QD (i.e., closed boundary surface dividing the QD and barrier regions), in this study, we consider the cubically shaped QDs with lengthLQD = 9 nm for simplicity, aiming at obtaining two IBs. Although the shape of the experimentally obtained QD is similar to a trapezoidal or a pyramidal shape, even a sim- pler geometrical shape can capture the essence of the physics in QDSLs as reported in Refs.27, 28). This is especially true for this study, because our focus here is to qualitatively elucidate the effect of IB wave-function localization on the SC efficiency for the case of multiple IBs. Therefore, a study based on a sim- ple QD shape is meaningful. The impact of the QD shape on the efficiency will be studied in detail in the future research.
1 2 3 4 5 6 7 8 9 10 0.0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0
Double degenerated states
1 2 3 4 5 6 7 8 9 10 0.00
Figure 2:(a) Energyeigenvalues are plotted as a function of the inter- QD separation The third group of eigenstates will be formed above the CB edge. (b) Tight-binding hopping energies for the first and second IBs are plotted as a function of the inter-QD separation.
2.2. Study of two QDs
As the first step of our analysis, we consider a model consisting of two cubic InAs QDs with the inter-QD separation smaller than 10 nm surrounded by a GaAs region with the side lengths Lz = 2 × dz + 2 × LQD along thez (stacking) direction and Lx(y) = LQD + dx(y) along the transverse direction, where
A. Mehdipour/Memoirs of the Graduate Schools of Engineering and System Informatics Kobe University, Vol. 6, 18-24 (2014)